Asymmetric poly(ethylene-alt-propylene)-poly(ethylene oxide) micelles:
A system with starlike morphology and interactions
M. Laurati,1,*J. Stellbrink,1R. Lund,1,†L. Willner,1E. Zaccarelli,2 and D. Richter1 1Institut für Festkörperforschung, Forschungszentrum Jülich, 52425 Jülich, Germany
2Dipartimento di Fisica and INFM-CRS SOFT, Università di Roma La Sapienza, Piazza A. Moro 2, I-00185, Roma, Italy
共Received 4 May 2007; published 18 October 2007兲
We report on an experimental study of single particle properties and interactions of poly 共ethylene-alt-propylene兲-poly共ethylene oxide兲 共PEP-PEO兲 starlike micelles. The starlike regime is achieved by an extremely asymmetric block ratio共1:20兲 and the number of arms 共functionality兲 is changed by varying the composition of the solvent共the interfacial tension兲. Small angle neutron scattering 共SANS兲 data in the dilute regime can be modeled by assuming a constant density profile in the micellar core 共compact core兲 and a starlike density profile in the corona共starlike shell兲. The starlike morphology of the corona is confirmed by a direct comparison with SANS measurements of dilute poly butadiene star solutions. Comparison of structure factors obtained by SANS measurements in the concentrated regime shows in addition that the interactions in the two systems are equivalent. Micellar structure factors at several packing fractions can be modeled by using the ultrasoft potential recently proposed for star polymers关Likos et al., Phys. Rev. Lett. 80, 4450 共1998兲兴. The experimental phase diagram of PEP-PEO micelles is quantitatively compared to theoretical expectations, finding good agreement for the location of the liquid-solid boundary and excellent agreement for the critical packing fraction where the liquid-to-bcc crystal transition takes place for f⬍70. The functionality, i.e., the coronal density, strongly influences the nature of the solid phase: for f⬍70 the system crystallizes into a bcc phase, high f ⬎70 formation of amorphous arrested states prevents crystallization.
DOI:10.1103/PhysRevE.76.041503 PACS number共s兲: 64.70.Nd, 61.12.Ex, 61.25.Hq, 82.35.Jk
Star polymers constitute a natural bridge between linear polymer chains and hard sphere colloids关2兴. Their softness is
controlled by the functionality f, i.e., the number of polymer chains tethered to the central microscopic core. For f = 2 the morphology of the star is that of a linear polymer chain while for very large f it resembles a spherical colloidal particle. This adjustable softness affects morphology as well as star-star interactions. The effective interaction potential intro-duced by Likos et al.关1兴 presents a logarithmic dependence
of the repulsion between two stars as a function of the center-to-center distance共r兲, for values of r smaller than the particle diameter. The strength of the repulsion is increasing with f and in the limit of f→⬁ the hard sphere potential is recovered. Such a potential was shown to give a correct de-scription of small angle neutron scattering 共SANS兲 data of star polymer solutions关1,3兴, while the hard-sphere
interac-tion potential failed 关4兴. Starting from the potential of Ref.
关1兴, the phase diagram of star polymer solutions was
calcu-lated, as a function of f and packing fraction 关5兴. Due to
the unusual soft repulsion between stars, a variety of equi-librium crystalline phases were predicted depending on and f. Recently the occurrence of nonequilibrium states was also taken into account. The mode-coupling theory共MCT兲 ideal glass transition line was found to closely track the
fluid-solid boundary in the equilibrium phase diagram关6兴.
Experimental investigation of star polymer solutions as a function of concentration and functionality f was qualita-tively confirming some of the features predicted by theory 关3,4,7兴, e.g., the formation of solid phases with increasing
polymer volume fraction . Concerning the nature of the solid phases observed at high volume fractions, there was little evidence of crystalline phases 关body-centered-cubic 共bcc兲 关8兴 and face-centered-cubic 共fcc兲 关8,9兴 at large f
val-ues兴, while in many cases the system was found to be trapped in a metastable arrested state 关3,7,10兴. However, a
systematic investigation of the experimental phase diagram of star polymers and a quantitative comparison with theory is still missing.
One of the main problems is that the high interest in star polymers is not reflected in their availability. Synthesis re-quires considerable preparative efforts and due to the den-drimer nature of the star core, the functionality f cannot be smoothly adjusted 关2兴. It would then be preferable to use a
readily available model system for star polymers that should not only show the typical molecular architecture of a star, but also interact via the effective potential proposed for star polymers. A natural candidate for such a model system is diblock copolymer micelles. A major task in a micellar sys-tem is that of approaching the starlike regime关11,12兴 defined
by the block ratio Na/ Nb1, with Na/ Nb the degrees of polymerization of the soluble-insoluble block. In fact very few block copolymers with asymmetric composition self-assemble into micellar structures since an extreme incompat-ibility between the blocks and between insoluble block and solvent is required. Two micellar systems turned out to be ideal in this respect: hydrophobically modified poly共ethylene oxide兲 PEO 关13–15兴 in water and asymmetric
poly共ethylene-*Present address: Lehrstuhl für Physik der Weichen Materie, IPkM, Heinrich-Heine Universität Düsseldorf, 40225 Düsseldorf, Germany; firstname.lastname@example.org
Present address: Donostia International Physics Center, Paseo Manuel de Lardizabal 4, 20018 San Sebastián, Spain.
alt-propylene兲-poly共ethylene oxide兲 共PEP-PEO兲 block co-polymers in water and water/N,N-dimethylformamide 共DMF兲 mixtures 关16,17兴. These systems form micelles with
small micellar cores and large extended coronas typical for starlike morphologies. The aggregation numbers are in the range between 30 and 130 ideally matching the functionality of regular star polymers accessible by living anionic poly-merization.
With regard to interactions, a few block copolymer micel-lar systems have been related to star polymers, even though in all cases the starlike regime was not achieved. In their pioneering work, Gast et al. investigated the dependence on block composition共0.8ⱕNa/ Nbⱕ4兲 of the lattice geometry 共fcc or bcc兲 of crystalline phases of poly共styrene兲-poly共isoprene兲 共PS-PI兲 block copolymers 关18兴. They found
that increasing block ratio, i.e., increasing the repulsion range, the bcc crystalline phase is stabilized against the fcc phase, in analogy to what is predicted for a reduction of the star functionality f. More recently bcc and fcc phases were observed in PS-PI 关19,20兴 and poly共ethylene
oxide兲-poly共butylene oxide兲 共PEO-PBO兲 关21兴 micelles. In both
cases, temperature was used as a control parameter for the transition between these two crystalline lattices. In Ref.关20兴
temperature changes were shown to induce variation of the aggregation number f and the fcc-bcc transition was com-pared to the phase diagram of star polymers, indicating some similarities in the interactions. However, the block ratio was rather small, Na/ Nb⬇2 关20兴.
In the present study we utilize PEP-PEO micelles pre-pared from block copolymers of very asymmetric composi-tion 共Na/ Nb⬇20兲 in aqueous solution as a star model sys-tem. Single particle properties and interactions were systematically investigated by SANS covering a broad con-centration range. The results are successfully compared to theoretical predictions for regular star polymers. The starlike nature of the system is confirmed by a direct comparison to experimental SANS data for polybutadiene 共PB兲 star poly-mer solutions in the dilute and concentrated regime. The functionality f of PEP-PEO can be effectively tuned by the addition of DMF allowing one to study the star polymers phase diagram over a broad range of functionalities f and volume fractions.
The results for single particle properties will be presented first in Sec. III A. The SANS measurements were performed at low concentrations. The PEO-block has been selectively deuterated, such that the micellar structure could be studied by individual contrasts 共core contrast, shell contrast兲. This allows an accurate determination of micellar functionalities 共core contrast兲 and verification of the starlike morphology of the micelles共shell contrast兲.
Subsequently, in Sec. III B, on the basis of experimental structure factors obtained from SANS measurements, we show the comparison between interactions of PEP-PEO mi-celles and of PB real star polymers. In Sec. III C the experi-mental phase diagram of PEP-PEO micelles is presented and discussed in terms of the theoretical phase diagram of star polymer solutions. Quantitative comparison to theory was obtained by modeling experimental structure factors S共Q兲, starting from the ultrasoft potential of Ref.关1兴. The
param-eters controlling the interaction, , f, and the interaction
length were directly given by experimental values. We illustrate how experimental data for PEP-PEO micelles re-produce to a high level of accuracy the liquid-solid transition of the theoretical phase diagram 共Sec. III C兲. Moreover, in agreement with theory, we show that f and thus the chain density of the micellar corona strongly influences the possi-bility for the system to crystallize. Concerning crystalline phases, we show that on the basis of simple arguments a heterogeneous crystalline structure is expected. Part of the results shown here have been presented in a recent paper 关22兴.
II. EXPERIMENTAL METHODS A. Micellar properties and sample preparation
The micellization behavior of PEP-PEO in aqueous solu-tion is governed by the large interfacial tension, ␥ = 46 mN/ m, between PEP and water. Such behavior was thoroughly studied by us during the last years关16,23兴,
result-ing in the followresult-ing findresult-ings. 共i兲 PEP-PEO forms micelles with the hydrophobic PEP constituting the core and the hy-drophilic PEO constituting the corona.共ii兲 Micelles are even formed in a very asymmetric block composition with high PEO content共Na/ Nb⬇20兲. 共iii兲 All micellar cores are com-pletely segregated, i.e., not swollen by solvent.共iv兲 The mi-celles are kinetically frozen in water: Although chemically not linked, exchange of block copolymers between different micelles could not be observed, not even at elevated tem-peratures 关24–26兴. This means that no free chains, i.e., no
depletion effects关7兴 are present. 共v兲 Adjusting␥by addition of a PEO selective cosolvent like N,N-dimethylformamide 共DMF兲 allows one to smoothly vary f even in the starlike regime共where f ⬃␥6/5was confirmed by experiments关17兴兲. Recent measurements of exchange kinetics in water/DMF mixtures 关25,26兴 observed significant block copolymers
ex-change at a DMF mole fraction共xDMF兲 larger than 0.4. The relatively high interfacial tension measured at xDMF= 0.4 关24–26兴, ␥= 16.5 mN/ m, indicates that despite the signifi-cant block copolymer exchange, the amount of free chains in solution should not induce significant depletion effects.
The asymmetric PEP-PEO block copolymer under study was synthesized by anionic polymerization关23兴. To exploit
h / d-contrast variation in our SANS experiments, the
indi-vidual blocks have been selectively protonated-deuterated, see Table I. The partial deuteration of the PEO chain was obtained by premixing deuterated and protonated EO mono-mers prior to the polymerization, leading to a copolymer with a random distribution of h- and d-repeat units. The
deu-TABLE I. Characterization of PEP-PEO block copolymer. Dpis the degree of polymerization, xhthe mole fraction of h-monomer, and the scattering length densities of polymer blocks.
Mn MW/ Mn Dp xh 关1010cm−2兴
PEP共block兲 1100 1.06 15 1.0 −0.31
PEO共block兲 20700 1.04a 436 0.11 6.32
teration degree was calculated from the initial amounts of h and d materials. The block copolymer and related PEP-OH parent materials were characterized by a combination of size exclusion cromatography 共SEC兲, 1H-NMR, and end group analysis关17,23兴.
Scattering length densities of the single blocks were cal-culated according to
with i indicating the PEP or PEO monomer,兺jbjthe sum of the coherent scattering lengths of all atoms in monomer i, andvithe average volume of one molecule of monomer i:
with Mi the molar mass of component i and ␦i the corre-sponding density.
The density of the PEP block was taken from关24兴, where
it was measured by means of an Anton Paar DMA 5000 density meter. The density␦of the PEO block was estimated using relation ␦hd PEO = 0.89␦d PEO + 0.11␦h PEO
, where the bulk density of h-PEO共␦h
PEO兲 was taken from 关
27兴 and the density
PEO兲 was calculated from that of the hydrogen-ated material by assuming identical volume.
Using water/DMF mixtures we prepared samples with six different f going from dilute 共0.25⫻10−2 polymer volume fraction兲 to the very concentrated regime 共up to ⬇0.27 poly-mer volume fraction兲. Binary mixtures of H2O / D2O and quaternary mixtures of H2O / D2O / DMF/ d-DMF with differ-ent volume fractions of the compondiffer-ents have been prepared for different contrast conditions. Water/DMF mixtures were found to be nonideal关17兴. Therefore the average densities of
the H2O / DMF and D2O / d-DMF mixtures were separately measured with an Anton Paar DMA 5000 density meter. The average scattering length densities of the hydrogenated 共h−mixt兲 and deuterated 共d−mixt兲 mixtures were calculated as described in关17兴. Finally the scattering length density of the
quaternary mixtures共0兲 were calculated using the additive relation0=h−mixth−mixt+d−mixtd−mixt. Values of0for the different solvent mixtures are listed in TableII.
The preparation of dilute solutions was already described in detail elsewhere 关17兴. Concentrated solutions were
pre-pared by mixing weighted amounts of solvent and polymer. Solvents were filtrated two times through Anotop membrane filters of 20 nm pore size. Samples were prepared separately directly in the measurement cells. The stability of the aggre-gation number of the micelles in the different samples was crosschecked in the SANS measurements, as will be shown later in the paper共Sec. II B 1兲. To homogenize the samples magnetic stirring balls of 0.5 and 1 mm diameter were intro-duced inside the cells and moved by applying an external weak magnetic field. After homogenization, samples were left at rest for at least 12 h共a few days in most of the cases兲 in order to equilibrate.
B. SANS experiments
Small angle neutron scattering experiments have been performed at KWS-1 and KWS-2 instruments 共Forschung-szentrum Jülich兲, at PAXY 共Laboratoire Leon Brillouin兲, at D11共Institute Laue Langevin兲, and at SANS-I 共Paul Scherrer Institut兲. Details about different setups and instrument speci-fications can be found in 关28兴. SANS data were corrected
following standard procedures and normalized to absolute units to allow a quantitative theoretical interpretation 共see, for example,关29兴兲.
The macroscopic scattering cross section, 共d⌺/d⍀兲共Q兲, measured by SANS can be expressed, for monodisperse par-ticles with spherical symmetry, as a product of single particle contributions, the particle form factor P共Q兲, and the structure factor S共Q兲, which contains all information about particle interactions:
冊共Q兲 = NzP共Q兲S共Q兲, 共3兲 Q =共4/兲sin共/ 2兲 is the modulus of the scattering vector
Q, defined as Q = ki− kswhere ki is the wave vector of the
incoming neutrons and ksis the wave vector of the scattered neutrons. is the neutron wavelength andis the scattering angle. Here Nz is the number density of particles. In the following we will refer to the scattering cross section as SANS intensity and we will use the nomenclature I共Q兲.
We measured particle form factors in dilute solution for all different solvent mixtures. Adjusting the scattering length density0of the solvent by use of h / d-isotopic mixtures to that of the PEO/PEP reduces the contrast factor between corona/core and solvent to zero, see TableII. Therefore core form factors and corona form factors were independently measured.
Experimental S共Q兲 can be extracted from SANS data measured in concentrated solutions by dividing out the ex-perimental P共Q兲 measured in dilute solution. However, this procedure is only valid if particle size and shape, i.e., P共Q兲, are unaffected by concentration. This is in general not the
TABLE II. Characterization of PEP-PEO micelles. xDMFis the mole fraction of DMF in the solvent and0is the scattering length density of the solvent. Rc,minand fminare the core radius and func-tionality from minimum position, Rc,fitand ffitare the core radius and functionality from fit to the compact core model, and Rmis the micellar radius obtained from fit to the core-shell model.
xDMF 0 共1010cm−2兲 Rc,min 共Å兲 fmin Rc,fit 共Å兲 ffit Rm 共Å兲 0.0 6.33 42 136 42± 1 140± 10 288± 12 0.1 6.32 37 94 36.4± 0.5 91± 4 265± 13 0.2 6.34 35 82 35.1± 0.5 83± 3.5 243± 12 0.3 6.33 34 73 33.8± 0.4 74± 3 222± 10 0.4 6.31 33 67 32.8± 0.5 68± 3 208± 6 0.5 6.31 32 63 32.5± 0.4 66± 2 200± 7
case for deformable particles like micelles. Moreover, fol-lowing the approach of Kotlarchyk and Chen for polydis-perse particles关30兴, it has been shown in recent studies that
for block copolymer micelles the factorization of the scatter-ing intensity into a form and structure factor followscatter-ing Eq. 共3兲 in general does not hold due to lack of spherical
symme-try of the micellar corona关31兴; but we can overcome these
problems by performing SANS experiments for concentrated solutions in core contrast only. Indeed the PEP core is com-pact, spherically symmetric, and completely unaffected by increasing concentration. The validity of this assumption can be rationalized from Fig.6, where the minimum arising from the solid core appears, at each fixed value of f, at the same Q value共within error bars兲 independent of, i.e., the core form factor is unchanged with increasing.
2. Theoretical models
Form factor. During the last years several different models for describing form factors of diblock copolymer micelles have been proposed. A recent review of the different models can be found in 关32,33兴. A very accurate model has been
recently proposed by Svaneborg and Pedersen, where short-range correlations and excluded volume interactions between chains in the corona have been quantitatively taken into ac-count关31,34兴. In the brush regime, the block copolymer
mi-celles can be alternatively modeled as a core-shell structure 关35兴, with a homogeneous density profile in the core and a
starlike density profile in the shell. The scattering contribu-tion of the corona chains, “blob scattering,” has to be imple-mented as an additional term using the Beaucage function 关36兴. Such an empirical model has been successfully used in
previous studies to describe scattering data from PEP-PEO micelles in water and water/DMF mixtures关16,17兴.
The scattering intensity measured in the dilute regime, in a generic contrast, was modeled according to the following expression:
I共Q兲 = NzP共Q兲 + Iblob共Q兲, 共4兲 where Iblob共Q兲 is the contribution due to the correlations be-tween the chains in the micellar corona, the so-called blob scattering, see Eq.共11兲. The micellar form factor P共Q兲 was
expressed as the ensemble average of the squared scattering amplitude A共Q兲:
P共Q兲 = 具兩A共Q兲兩2典. 共5兲
The scattering amplitude of micelles formed by a compact PEP core and a diffuse PEO corona was described using a spherical core-shell model, according to the following rela-tion关16,23兴:
A共Q兲 = 共c−0兲VcA共Q兲c+共sh−0兲VshA共Q兲sh, 共6兲 where Vc and Vsh are the core volume and the corona vol-ume, respectively. A共Q兲c and A共Q兲sh denote the core and shell scattering amplitudes. The partial scattering amplitudes of core and shell in spherical symmetry can be written as the Fourier transform of the radial density distribution, n共r兲 关16兴:
A共Q兲c,sh= 1 C
冕0 ⬁ 4r2n共r兲sin共Qr兲 Qr dr, 共7兲 with C =兰0⬁n共r兲4r2dr.
The radial density distribution in the core was assumed to be constant. The possible presence of surface roughness or a diffuse interface between core and corona were taken into account by convoluting the density distribution with a Gaussian distribution function, leading to
3 sin共QRc兲 − QRccos共QRc兲 共QRc兲2
exp关− 共cQ兲2/4兴, 共8兲 where c is the smearing parameter. Here Rc is the core radius, given by Rc=
冊1/3 . 共9兲
It was assumed a compact, solvent, and PEO free core with a total volume Vc= fVPEP, where VPEPis the volume of a PEP chain.
The shell was described using a hyperbolic distribution, combined with a Fermi function in order to have a cutoff of the power law dependence, according to the finite size of the polymer chain关16兴.
n共r兲 = r
1 + exp关共r − Rm兲/共mRm兲兴
with Rm the overall micellar radius and m the smearing parameter that adjusts the cutoff distance of the Fermi tion. The value 4 / 3 for the exponent of the hyperbolic func-tion is typical for starlike structures关16兴.
As anticipated, in order to describe blob scattering contri-butions to the scattering cross section we used the Beaucage function关36兴: Iblob共Q兲 = 共sh−0兲2B
冊D , 共11兲
where erf is the error function, B is an intensity prefactor proportional to the blob volume,is the blob radius, and D the fractal dimension of the object.
Structure factor. Pair correlation functions g共r兲, where r is the distance between the centers of two particles, were cal-culated by solving the Ornstein-Zernike integral equation with the Rogers-Young共RY兲 closure relation 关37兴:
g共r兲 = exp关−␤v共r兲兴
冋1 +exp兵f共r兲关h共r兲 − c共r兲兴 − 1其
共12兲 where␤= 1 / kBT, v共r兲 is the pair interaction potential, h共r兲 = g共r兲−1 is the total correlation function, c共r兲 is the direct correlation function, and f共r兲=1−exp共−␣r兲. The parameter ␣ is used to achieve thermodynamic consistency. The RY closure relation was shown to give satisfactory agreement with simulations for many repulsive types of interactions, including star polymers 关38,39兴, star polymer mixtures
关40,41兴, square shoulder 关42兴, and ramp potentials 关43兴.
In Eq.共12兲 the ultrasoft potential of Ref. 关1兴 was used. For
clarity we report the potential form here: ␤V共r兲 = 5 18f 3/2
冊+ 1 1 +
册, rⱕ = 5 18f 3/2 /r 1 +
冑f共r −兲 2
册, rⱖ, 共13兲 where is the interaction length, defined as the distance between two star centers, when the outermost blobs in the corona fully overlap. Theoretical structure factors were fi-nally obtained by Fourier transformation of the pair correla-tion funccorrela-tions g共r兲:
S共Q兲 = 1 +N
冕dr exp共iQ · r兲关g共r兲 − 1兴. 共14兲 III. RESULTS AND DISCUSSION
A. Form factor and single particle properties
In this section results concerning single particle proper-ties, i.e., form factors P共Q兲, will be presented. The micellar characterization was aiming at determining共i兲 the function-ality f, as a function of DMF content of the solvent and共ii兲 the size of the core and corona of the micelles. Furthermore, the density distribution of the micellar corona was tested against Eq.共10兲 in order to verify the starlike morphology of
Form factors P共Q兲 have been measured in core and shell 共corona兲 contrast conditions as a function of the DMF con-tent of the solvent. For core contrast studies the polymer volume fraction in solution was in all cases⬇0.25⫻10−2. The desired scattering length density for core contrast con-dition was, in a first step, assumed to equal the scattering length density of PEO as calculated for TableI. Furthermore, since we could not exclude small uncertainties in chemical composition of h / d material along the polymer chain and possible deviations of the density of PEO in solution as com-pared to bulk关24,44,45兴, the core-contrast condition was
de-termined in an experiment where the scattering length den-sity of the solvent was changed starting from the fully deuterated solvent and adding step-by-step a droplet of hy-drogenated solvent by using a Hamilton 10l syringe, until no contribution from the corona could be detected. Figure1
shows the SANS intensities measured at 8 m sample to de-tector distance. Intensities have been normalized to the poly-mer volume fraction . Starting from the sample in pure D2O, the forward scattering 关I共Q→0兲兴 in the range 10−2Å−1⬍Q⬍2⫻10−2Å−1 shows an upturn which de-creases with the addition of H2O until a plateau is reached after the third addition, corresponding to a D2O volume frac-tion in the solventD
2O= 0.981. Here the core contrast
con-dition is achieved, providing a value of the scattering length density of the matching solventcc= 6.31⫻1010cm−2. Fur-ther increasing the H2O amount produces a downturn of the
forward scattering, meaning that the scattering length density of the solvent became smaller than that of PEO. In this case according to Eq.共6兲 the cross term in 兩A共Q兲兩2becomes nega-tive changing the upturn of the forward scattering into a downturn. Additional details on this experiment can be found in关28兴.
The core radius Rc and the functionality f can be esti-mated from the position of the minimum in the form factor. Indeed, assuming a homogeneous compact spherical core, the form factor has its first minimum at
QRc⬇ 4.49. 共15兲
Once obtained, Rc from Eq. 共15兲, f derive from Eq. 共9兲. Exemplary experimental core contrast form factors measured for two solvents with different DMF mole fraction, xDMF = 0.2 and 0.5, are reported in Fig.2共a兲. Qualitatively, by com-paring the two form factors, it is evident that the position of the minimum is moving towards higher Q values with in-creasing DMF content. According to Eq. 共15兲, this means
that Rcis decreasing with increasing DMF content, and cor-respondingly the functionality f. The reduction of f is con-firmed by the reduced value of the forward scattering with increasing DMF content. Values of Rcand f obtained from the minimum position for all solvents are listed in TableII.
Figure 2共a兲 shows also fits to the compact core model described in Eqs. 共5兲, 共6兲, and 共8兲. In the fit, the effect of
experimental resolution was included, by convoluting the model function with the resolution function, as described in 关46兴. It should be noticed that since the resolution is different
for the different instrumental setups used to cover the entire
Q range of data, the original fitted curves were composed of
separated parts corresponding to each setup. In order to make the plots more clear, we decided to present them as a con-tinuous curve instead of separated into parts. The only ad-justable parameter in the fit was the core radius Rc. The functionality f is obtained from Rcaccording to Eq.共9兲. This also means that a good fit is obtained when both minimum position and forward scattering provide the same value of f. The small deviations between fitted curves and experimental
120 115 110 105 100 95 90 I(Q)/ φ [cm -1] 22x10-3 20 18 16 14 12 Q[Å-1]
FIG. 1. SANS intensities from dilute PEP-PEO micellar solu-tions in H2O / D2O mixtures. The intensities are normalized to poly-mer volume fraction . The D2O volume fraction in the solvent
共D2O兲 is 共⽧兲 pure D2O, D2O= 0.999, 共䊊兲 D2O= 0.991, 共䊏兲
D2O= 0.985,共䉭兲 D2O= 0.981, 共䉲兲D2O= 0.978, and 共〫兲 D2O
data observable around the minimum could arise from small polydispersity effects which would not seriously change the obtained values of Rc.
Additionally, experimental data for xDMF= 0.2 show some excess scattering in the region of Qⱕ3⫻10−2Å−1that is not properly modeled. Such an excess scattering is most likely due to undesired instrumental effects, like an imperfect beam alignment. Such effects could be significant in the case of core-contrast form factors, since in such a contrast condition only a small part of the particle contributes to the coherent scattering共the small PEP core兲, therefore the overall scatter-ing from the particles in a dilute solution is quite small com-pared to the overall scattering. Alternatively, the excess scat-tering could be attributed to residual shell contributions or to the presence of large scale structures, like clusters, in solu-tion. We postpone the discussion of the last two effects to the section about interactions, since excess scattering was ob-served also in concentrated solutions. Values of Rc and f obtained from fits are also reported in TableII. The agree-ment with the set of results obtained from the minimum po-sition is satisfactory.
Form factors in shell contrast condition are shown in Fig.
2共b兲 for the solvents xDMF= 0.2 and 0.5. It can be noticed that, also in shell contrast, the forward scattering 关I共Q
→0兲兴 is decreasing with increasing DMF content,
confirm-ing the reduction of the micellar functionality. For Q ⱖ0.03 Å−1 the data show a clear power law dependence, which was found to be approximately I共Q兲⬃Q−1.4. For swol-len polymer chains in good solvent condition a power law
dependence I共Q兲⬃Q−1.7is expected on the basis of the Flory exponent= 0.588 and the fact that at high values of Q the scattering intensity from an object with fractal dimension D scales as I共Q兲⬃Q−D, where D = 1 / 关47兴. The experimental value is smaller, in agreement with previous SANS experi-ments on PI and PB star polymers 关I共Q兲⬃Q−1.5兴 关48–50兴, where the larger value of was attributed to a stretched configuration of the chains in star polymers due to geometric-steric constraints. Data were modeled according to the core-shell model of Eqs.共5兲 and 共6兲, assuming a starlike
density distribution of the micellar corona according to Eq. 共10兲. In order to stabilize the values of Rm in the fits, the smearing parameter of the Fermi function, m, was kept fixed at 10% of the micellar radius, according to previous investigations of asymmetric PEP-PEO micelles关16兴. Since
for us the parameter of interest in the modeling was the mi-cellar radius Rm, we did not go in depth using a microscopic description of the blob scattering, therefore we used the Beaucage function described in Eq.共11兲 to model the
scat-tering intensity at high Q. Blob intensity prefactors were found to be of order 10−23cm3, the blob size was varying in the range= 60– 80 Å, while the fractal exponent was found to be approximately D = 1.4 in all cases. Values of Rm ob-tained from fits are reported in TableII. The obtained values show a contraction of the micellar corona with increasing DMF content, consistent with the decrease of the second virial coefficient A2 with increasing DMF content observed in Ref. 关17兴. The decreasing functionality with increasing
DMF content could only contribute slightly to the contrac-tion of the micellar corona. Indeed let us define the reduced surface covering of the micellar core according to 关34兴,
red=共fRg02 兲/4共Rc+ Rg0兲2, where Rg0 is the radius of gy-ration of a chain in the micellar corona. If one calculatesred using the values of Rcfrom Table II and of Rg0from Ref. 关17兴, one obtains a decrease from red= 14 at xDMF= 0 to red= 8 at xDMF= 0.5, which means that the corona is still in the brush regime共red1兲.
The good quality of the fits, based on the starlike profile of Eq.共10兲, confirms the starlike architecture of the micellar
The starlike morphology of the micelles was also directly verified by a comparison to the form factor of PB star poly-mers with nominal functionality f = 64, as shown in Fig. 3. The Q vectors of the two data sets were rescaled to the respective radii of gyration, Rg= 135 Å for the micelles ac-cording to TableIIand Rg= 44.3 Å for the PB stars关3兴. The SANS intensities were rescaled to the respective volume fractions, contrast 共⌬2兲, and molecular volumes 共V
w兲 of polymer chains. The two curves accurately overlap in the whole Q-range, thus confirming the starlike morphology of PEP-PEO micelles.
The starlike features of the micellar corona can be empha-sized by using a generalized Kratky representation of the data, i.e., by plotting I共Q兲Q1/ vs Q. For branched polymers like star polymers, this representation shows a characteristic peak whose height reduces with decreasing functionality. This behavior was experimentally observed for star polymers 关48兴. Figure4shows shell contrast form factors correspond-ing to different values of xDMFin generalized Kratky
repre-10-1 100 101 102
]0.01 2 3 4 5 6 7 8 90.1 2
]xDMF= 0.2 xDMF= 0.5
fit compact sphere
100 101 102 103
]2 3 4 5 6 7 8 9 0.01 2 3 4 5 6 7 8 90.1
]Q-1.4 xDMF= 0.2 xDMF= 0.5
fit star-like shell
FIG. 2.共Color online兲 共a兲 Experimental core contrast form fac-tors for xDMF= 0.2 and 0.5 solvent mixtures and fits to compact core model.共b兲 Experimental shell contrast form factors and fits to core-shell model; green line: Q−1.4scaling of I共Q兲 in the high Q range.
sentation, where 1 / has chosen to be equal to 1.4. A clear characteristic peak is present, whose height is strongly de-creasing from pure water to xDMF= 0.5, corresponding to the reduction of micellar functionality. Data are merging into a plateau in the region of higher Q, which corresponds to the regime where Q−1.4scaling of intensities was observed. The inset of Fig. 4 presents, in Kratky representation, the com-parison between the form factor of PEP-PEO micelles with
f = 63 and the form factor of PB stars with nominal f = 64.
The Kratky representation provides an additional indepen-dent way to estimate the radius of gyration of the micelles. In the region around the peak, the form factor can be approxi-mated by the Gaussian star form factor of Benoit关51兴:
P共Q兲 = 2 fv4
冉v 2−关1 − exp共− v2兲兴 + f − 1 2 关1 − exp共− v 2兲兴2
冊, 共16兲 where v =
冑f/共3f − 2兲QRg. 共17兲 This form factor is in principle describing star polymers un-der ⌰ solvent conditions, but excluded volume effects for swollen chains are not affecting the Q range around the peak.
The position of the maximum of the Benoit form factor,vmax, can be calculated from the first derivative of expression共16兲
with respect tov, for each value of the functionality f, fixed
to the experimental values of TableII. Values ofvmaxin the range vmax= 0.94– 1.01 were found depending on f. Using these values and positions of the maximum from experimen-tal data of Fig. 4, the micellar radius of gyration Rg was estimated for each functionality. Values of Rgobtained from the Benoit model applied to form factors in Kratky represen-tation are listed in Table III. Values of Rg from the Benoit model are in good agreement with values independently ob-tained from the core-shell model and interaction length 共next section兲.
On the basis of the results of characterization of PEP-PEO micelles in dilute solution and comparison to regular star polymers, we can conclude that for what concerns internal structure and morphology, our micellar system can be de-scribed as a starlike system where the functionality can be easily adjusted through changes in solvent composition.
B. Structure factor and interactions
Interactions between micelles were investigated through interparticle structure factors S共Q兲 obtained by SANS. Ex-perimental structure factors for the six different functional-ities were extracted from SANS intensfunctional-ities measured in core contrast, as explained in Sec. II B 1. Structure factors for several values of polymer volume fraction have been mea-sured for each functionality. A direct connection between in-teractions in PEP-PEO micelles and in regular star polymers was obtained by comparing structure factors obtained for mi-celles with f = 63 共water/DMF mixture with molar fraction
xDMF= 0.5兲 and a corresponding PB star polymer in methyl-cyclohexane with 共nominal兲 64 arms 关3兴. Structure factors
measured at different values of the ratio /* have been compared, with*= 3 /共4R
w/¯N␦ A兲 being the
over-10-3 10-2 10-1 100 I(Q)/ φ(∆ρ) 2 V w 2 3 4 5 6 7 8 9 1 2 3 4 5 6 7 8 910 QRg
FIG. 3.共Color online兲 Comparison between shell contrast form factor of PEP-PEO micelles with f = 63共closed symbol兲 and form factor of PB stars with nominal functionality f = 64共open symbol兲.
FIG. 4. 共Color online兲 Generalized Kratky representation of shell contrast form factors for different values of DMF content:共䉮兲 xDMF= 0.0,共䊐兲 xDMF= 0.1,共䉭兲 xDMF= 0.2, and共䊊兲 xDMF= 0.5. In-set: Kratky representation of form factors of PEP-PEO micelles with f = 63共closed symbol兲 and PB stars with f =64 共open symbol兲.
TABLE III. Left: Comparison between values for the radius of gyration obtained from structure factor modeling of solutions below *共R
兲, from form factor analysis 共Rg兲, and from the Benoit model applied to Kratky representation of shell-contrast form factors共Rgkr兲. Right: abccand asc values obtained from crystalline samples with f = 63共xDMF= 0.5兲 and different values of the packing fraction =共/6兲Nz3, where N
z is the particle number density and the interaction length. Values of 2Rm are reported for comparison. Analogous results, not shown here, were obtained for samples with f = 67共xDMF= 0.4兲. fbccvalues are calculated according to Eq.共20兲.
f R 共Å兲 Rg 共Å兲 Rgkr 共Å兲 a共Å兲bcc asc 共Å兲 2Rm 共Å兲 fbcc 63 127 140 144 0.21 381 270 377 82 67 136.5 145 148 0.23 367 260 375 82 73 140 155 155 0.24 367 260 372 90 82 154 169 166 0.26 341 241 368 81 94 161 184 198 0.28 341 241 362 91 136 192 200 202 0.31 330 233 356 94 0.41 309 218 336 112
lap volume fraction and ¯ the average density. Figure␦ 5
shows the comparison between structure factors of PEP-PEO micelles and PB star polymers for three values of, below, at and above the overlap volume fraction: The main features of the star S共Q兲 with respect to peak positions and heights are well-reproduced below and at the overlap volume frac-tion, as depicted in plots共a兲 and 共b兲 of Fig.5. The fact that a third peak in the region of large Q is observed for the micellar system but not for the PB star is due to the fact that for the PB star this peak is masked by the diffuse blob scat-tering of the polymer arms关31兴.
Above*, while the first peaks still overlap, differences evolve between the star and the PEP-PEO micelles for larger values of Q 关Fig. 5共c兲兴. In particular the S共Q兲 of the mi-celles presents an additional peak where the structure factor of the stars has the first minimum共6⬍Q⬍7兲. As it will be explained in more detail later, the observed additional peak in the micellar S共Q兲 is related to the formation of a crystal-line phase in the micellar system above*, not observed for the PB stars.
The larger width of the micellar S共Q兲 around the first peak can be attributed to the different resolution of the D11 spec-trometer 共6 Å wavelength, 10% wavelength spread, 1 ⫻1 cm2 detector pixel size, 30⫻30 mm2 squared collima-tion aperture, and 13 mm diameter of sample aperture兲, where micellar data have been measured, and of the PAXY spectrometer 共10 Å wavelength, 13% wavelength spread, 0.5⫻0.5 cm2 detector pixel size, 13 mm diameter of colli-mation aperture, and 7.6 mm diameter of sample aperture兲, where PB star data have been measured. In all three com-parisons, in the low Q region the micellar S共Q兲 shows some
increase indicating some excess scattering. Such excess scat-tering might arise either from共i兲 共inherent兲 mesoscopic het-erogeneities as also found in experiments with purely repul-sive star polymer solutions 关52,53兴 or 共ii兲 from weak
attractive interactions due to residual dispersion forces, i.e., decreasing solvent quality with increasing xDMF关17兴 or 共iii兲 residual contributions from the shell form factor.
In the first case, this result only further supports the anal-ogy between PEP-PEO micelles and star polymers. It should be noticed that the analogy refers to good solvent conditions but is not completely athermal, in agreement with the cited Refs.关52,53兴. Indeed, as one can see in Fig.5, no signature of such heterogeneities appear in PB star polymers in meth-ylcyclohexane, which is an athermal solvent for PB. In the second case, it has been shown that the presence of an at-tractive interaction共for example, of van der Waals type兲 in addition to the repulsive potential of Eq.共13兲 does not
sub-stantially influence the freezing and the glass transition of the system, if the width of the attraction well is sufficiently large 关39,54兴, while a shift of the MCT ideal glass transition line
towards larger packing fractions is expected for a shorter range of attraction 关54兴. Our results on the phase diagram,
presented later in this section, show that dynamical arrest in the system happens at volume fractions comparable or smaller than expected for purely repulsive star polymers, thus pointing in the direction of absence of attractive inter-actions, or presence of rather long-ranged attractive interac-tions in our system. Finally the presence of residual contri-butions from the shell in the low-Q range might arise from different mechanisms of water-heavy water adsorption around the soluble partially deuterated PEO block 关55–57兴.
The origins of such mechanisms are still under debate and a quantitative discussion of these effects on the basis of our data is under investigation. It has to be noted though that spurious contributions from the shell would not affect the range of Q where the structural features, i.e., peaks of the structure factor S共Q兲 appear, as also confirmed by the core contrast experiment of Sec. III A.
Excess scattering affects the low Q regime of all data from concentrated solutions, giving rise to a discrepancy be-tween experimental data and theory calculations in this re-gime. Here we will focus on the Q regime where the struc-tural features corresponding to pair interactions between single particles are present. As will be shown below on the basis of our analysis, whatever the origin of such excess scattering is, the low-Q scattering does not have major rel-evance on the quantitative interpretation of S共Q兲 for Q ⱖ10−2Å−1.
Interactions in PEP-PEO micellar solutions were also compared to theoretical predictions for regular star polymers. We will describe in detail the modeling procedure that was used to model SANS data from the investigated samples. It should be noticed here that, since we have shown that inter-actions in our system reproduce those of real star polymers, a description of the interactions on the basis of a hard-sphere potential was excluded from the beginning.
The modeling was obtained in a two-step procedure. In the first step, theoretical S共Q兲 were calculated, according to the procedure described in Sec. II B 2, for a fixed f and dif-ferent values of the packing fraction , that are calculated
3.0 2.0 1.0 0.0 S( Q) 16 14 12 10 8 6 4 Qσ 3.0 2.0 1.0 0.0 S( Q) 16 14 12 10 8 6 4 Qσ 3.0 2.0 1.0 0.0 S( Q) 16 14 12 10 8 6 4 Qσ
FIG. 5. S共Q兲 for PEP-PEO micelles with f =63 共closed symbols兲 compared to a 64-arm共nominal兲 PB star 共open symbols兲, at three different values of the ratio/*:共a兲/*⬇0.82, 共b兲 /*⬇1,
according to=共/ 6兲Nz3, where Nzis the particle number density. The obtained structure factors were compared to ex-perimental ones at fixed volume fraction by rescaling the theoretical Q abscissa to the experimental Q-range. This means that for each differentwe obtained a different value of. It has to be noticed that the experimental packing frac-tion in terms ofcannot be calculated a priori on the basis of the measurements, sincecan only be obtained by mod-eling the experimental structure factor. The second step con-sisted of determining the best description of the experimental structure factor among the selected theoretical ones. To do that, it was necessary to take into account the effect of ex-perimental resolution, which is affecting the peak height and width of the experimental S共Q兲.
Since the experimental S共Q兲 cannot be easily deluted from resolution effects, it is then preferable to convo-lute the theoretical model for the overall SANS coherent cross section I共Q兲⬃ P共Q兲S共Q兲 to the resolution function, as mentioned for the form factor analysis. For P共Q兲 we as-sumed the compact core model, fixing the parameters to f and Rcvalues obtained from the characterization of the mi-celles. The validity of this assumption was explained in Sec. II B 1. For each experimental I共Q兲, the selected different the-oretical structure factors, corresponding to different values of , were tested against experimental data. The result of com-parison between theory curves where resolution effects are taken into account and the measured cross section allows us to select the theoretical structure factor which gives the best description of the experimental data. The best description of the data is selected as the one where the height and width of the structural peaks is more accurately reproduced. From the
chosen theoretical structure factor the value offor a given experimental packing fraction is obtained.
Use of potential of Eq.共13兲 to calculate S共Q兲 was proven
to give satisfactory description of experimental data for the full range of functionalities and volume fractions measured. Examples of comparisons between theory and experiments are shown in Fig.6. In the same figure, in each single plot related to a fixed functionality f, it can be again observed that at all different volume fractions the position of the mini-mum of the form factor, visible in the range Qⱖ0.1 Å−1, does not change with increasing volume fraction, confirming the stability of the micellar morphology at all volume frac-tions.
Theparameter is defined in the theoretical model as the distance between the two star centers, when the outermost blobs in the corona fully overlap. The radius of this blob, from geometry, is simply Rb⬇/
冑f. Since below*the par-ticles do not overlap, a star radius can be defined as the half of plus the radius of the outermost blob:
R= 2 +
Using Eq.共18兲, Rwas calculated for all measured samples,
f was taken from the form factor analysis.
According to scaling theory, the size of a star should not be affected by concentration effects until the star coronas start to overlap关58兴. This means that below the overlap
vol-ume fraction*, R
should stay constant at fixed f. Values of
Robtained for samples below*are plotted as a function of
in Fig. 7, for all measured functionalities. As it can be
FIG. 6. Comparison between experimental SANS intensities共points兲 and theory 共lines兲 for four different functionalities: 共a兲 f =67, 共b兲 f = 73,共c兲 f =82, and 共d兲 f =94, and different volume fractions 共in legends兲. For clarity, in each plot intensities have been shifted with respect to the data with the smallest volume fraction.
noticed, in all cases data related to a single f value are dis-tributed with small deviations around an average value R, in agreement with scaling theory predictions. Moreover, data can be compared to the radius of gyration obtained in the very dilute regime, i.e., from the form factor analysis. From that analysis the micellar radius Rmwas obtained as the cut-off distance of the Fermi function for the starlike density profile in the corona, see Eq.共10兲. Rgcan be calculated from
Rmaccording to Rg2=
冕0 Rm n共r兲r4dr
冕0 Rm n共r兲r2dr , 共19兲
where n共r兲 corresponds to the expression in Eq. 共10兲. Values
of Rg are in good agreement with R, as it can be noticed from TableIII.
When the particles start to interpenetrate, the star coronas are shrinking. The Daoud-Cotton model predicts that the ra-dius of a star polymer scales as⬃−1/8with increasing poly-mer volume fraction above*关9,58兴. This scaling behavior was tested only for samples with f = 63, 67, and 136, where a sufficient number of samples above* were measured. For all three cases the agreement between experimental data and scaling theory predictions is excellent, as shown in Fig.7. It should be noticed that, while the range of volume fractions investigated is not large enough to fully establish scaling predictions, it is much larger than in previous studies of regular star polymers关48兴. We can conclude that the
interac-tion length obtained by describing experimental S共Q兲 via
the ultrasoft potential proposed for regular star polymers are within error bars quantitatively given by the molecular size of the single starlike PEP-PEO micelle.
C. Phase diagram
The values of obtained from comparison between theory and experiments have been used to recalculate the packing fraction from the given experimental particle number density Nz. The evaluation of is essential in order to compare the experimental and theoretical phase diagram. For ⬍* the average value of the interaction length dis-played in Fig. 7 was used, while for ⬎* we took the individual values of obtained for each separate volume fraction, sincevaries with.
Experimental points with coordinates共, f兲 were then lo-cated in the theoretical phase diagram of Ref.关5兴. The
result-ing diagram is presented in Fig.8. Good agreement between theory and experiments was obtained for the liquid-solid boundary in the whole range of functionalities and packing fractions. In particular the liquid-to-bcc crystal transition for
f⬍70 is perfectly reproduced experimentally. The packing
fraction for crystallization was found to bec⬇0.21. Experimental evidence for the formation of crystalline states comes from the observation of Bragg peaks in the two-dimensional 共2D兲 SANS pattern of the detector, as shown in Fig9. Moreover, structure factors of samples pre-senting Bragg peaks have a first peak which equals or ex-ceeds the minimum value for freezing transition, 2.8, pre-dicted by the Hansen-Verlet criterion关59兴. It should be noted
that the effect of experimental resolution is that of reducing the peak height, therefore the Hansen-Verlet criterion is cer-tainly fulfilled.
The crystalline lattice can be determined on the basis of the relative position of the first three peaks of the structure factor. It can be noticed that, corresponding to the onset of crystallization, an additional peak at intermediate distances appears in the structure factors, as shown in Fig.9. The peak ratio with respect to the first peak is 1 :
冑3, characteristic of a bcc or simple-cubic共sc兲 lattice 关60兴. The A15 lattice 关61兴
can be excluded, since its additional reflection at
冑5 / 2 was
200 180 160 140 120 Rσ [Å] 1.0 0.8 0.6 0.4 0.2 φ/φ∗ f = 63 f = 67 f = 73 f = 82 f = 94 f = 136 180 160 140 120 100 Rσ [Å] 5 4 3 2 1 φ/φ∗ f = 63 f = 67 f = 136
FIG. 7. Scaling behavior of Rwith for samples with polymer volume fraction below*共upper plot兲 and above*共lower plot兲.
For each f Ris constant below*and scales as−1/8above*.
FIG. 8. Experimental phase diagram共symbols兲 of starlike mi-celles vs theoretical phase diagram 共lines兲 of star polymers. 共䊊兲 liquid,共䊏兲 bcc crystal, and 共䉱兲 gels. The dashed line represents the equilibrium phase diagram from Ref.关5兴. The solid line is the
not observed. It is expected to occur in a region where the form factor is close to unity. In order to select between the bcc and the sc lattice, we calculated the lattice parameter a for the two options, abcc= 2
冑2 / Qmax and asc= 2/ Qmax. At the overlap volume fraction the lattice parameter should be equal to the double of the micellar radius Rm and decrease for larger volume fractions because particles start to inter-penetrate. This is the trend of abccwith increasing above * whereas the values of a
sc are always smaller than 2Rm, see Table III. Therefore the cubic lattice was identified as bcc.
Additionally it may be speculated that the ability of the system to crystallize for functionalities f⬍70 is connected to the significant copolymer exchange between micelles re-cently measured in time-resolved SANS measurements 关25,26兴. Probably, this facilitates the packing of micelles in
ordered structures with increasing volume fraction, as ob-served also for other micellar systems关62,63兴. It should be
noticed though that still the critical packing fraction for crys-tallization should be determined by the interaction potential between micelles at a specific functionality, when the func-tionality does not change with polymer volume fraction: In our case indeed the average micellar functionality is un-changed over the whole range of polymer volume fractions, as already shown from the stability of the form factor mini-mum共Fig.6兲, and we were able therefore to relate the
ob-served liquid-to-bcc crystal transition directly to the interac-tion potential predicted for star polymers.
Still considering the range of functionalities f⬍70, fur-ther increasing the polymer volume fraction in the solid phase we could not observe any evidence of transition to an fcc lattice. At the moment we are missing a clear explanation of this phenomenon. Theory predicts in this functionality range a rather small free energy difference between bcc and fcc lattices: for example, for f = 64 and = 0.5 the lattice energy sum for bcc is E / kBT = 94.65 and for fcc is E / kBT = 94.07关64兴. Such an energy difference is enough to stabilize
fcc against bcc, however, a metastable bcc phase could be formed as a precursor of the equilibrium fcc phase, according
to the Ostwald’s step rule关65兴. Such a metastable bcc phase
was observed for PS-PI micelles 关62兴 and it was shown to
have a lifetime of the order of hours.
In our experiments, solutions corresponding to packing fractions, where fcc lattices would be expected as equilib-rium states, were measured after a time period ranging from 1 to 2 weeks from sample preparation. Since only bcc phases were observed, this would mean that the lifetime of such a metastable state would be in our case at least longer than 2 weeks. A different explanation would be that of formation of mixed phases, consisting of equilibrium bcc crystalline re-gions containing a fraction of the total number of micelles and dynamically arrested regions containing the remaining particles. Far enough from the glass transition one would expect an almost homogeneous bcc crystalline phase, while increasing the packing fraction towards the glass transition more arrested regions should be formed. Formation of such a mixed phase would prevent the establishment of the under-lying equilibrium fcc phase. Such a speculation could be tested by checking the homogeneity of the crystalline bcc phases at packing fractions where an fcc phase would be expected. This could be done on the basis of simple geo-metrical considerations: In the case of a homogeneous bcc phase, the sample volume is given by the number of cubic cells times the volume of a cell共abcc3 兲. Since in a bcc crystal there are two particles per unit cell, the number of cells is simply half of the number of particles. For a monodisperse starlike micelle, each particle is constituted of f polymer chains, which means that the number of particles is equal to the number of polymers divided by f. Therefore we could recalculate the micellar functionality according to the rela-tion
where ␦PEP−PEO is the average polymer density. Values of functionality calculated according to Eq. 共20兲 for samples
with f = 63 and polymer volume fractions where fcc phases are expected are listed in TableIII. The values are in all cases significantly larger than those established on the basis of the form factor analysis. This suggests that the observed bcc crystalline phases are not homogeneous. Moreover, the dif-ference between the functionalities obtained from Eq. 共20兲
and those obtained from the form factor analysis is almost constant in the region far away from the glass transition, where bcc crystals are expected from theory, while it starts to increase in the region, approaching the glass transition, where fcc crystals are expected.
For f⬎70, when crossing the overlap volume fraction*, no crystals are formed. Indeed no Bragg peaks were ob-served in SANS measurements, and the obtained structure factors present first peaks that do not fulfill the Hansen-Verlet criterion, as shown in Fig. 10. Nevertheless for ⱖ*all samples were found to be in a solid state. Evidence for formation of solid, noncrystalline states for f⬎70 was obtained from tube inversion. By tube inversion we checked the tendency of the sample to flow: For all solid samples we could not observe any flow over a time scale of the order of
FIG. 9. 共Color online兲 Liquid 共open symbol,=0.072兲 to crys-tal共closed symbol,=0.091兲 transition observed for samples with f = 67: A structure factor above*presents a first peak larger than 2.8 and an additional second peak, the ratio between the three peaks is 1 :
冑3. Inset: Bragg peaks observed in a 2D SANS pattern of the detector, for f = 63 and=0.16.
a week. The temperature of the sample was kept constant by means of a liquid bath. Results of tube inversion experiments are supported by oscillatory rheology measurements per-formed for solutions of the analogous 共same block ratio兲 fully hydrogenated PEP-PEO block copolymer. The inset of Fig.10 shows results of dynamic frequency sweeps for two solutions of the hydrogenated PEP-PEO block copolymer in pure water共f =120兲, one slightly below the overlap volume fraction and one slightly above it. Below*the response is characteristic of a viscous fluid, with the loss modulus G
⬙larger than the storage modulus G
⬘and a determined fre-quency dependence. Above*one instead observes a typical solidlike response, with the storage modulus larger than the loss modulus.
Formation of disordered arrested states above the overlap volume fraction*for fⱖ70 has been also reported for PB stars关10,53兴. The dynamical arrest of the system was
attrib-uted to formation of clusters when the arms in the outermost blobs of the particles start to overlap. Indeed in case of a sufficiently large segment density in the corona, the geomet-ric confinement can strongly suppress the chain dynamics, leading to formation of geometric constraints and conse-quently of clusters. Even a small number of clusters could induce a macroscopically arrested state关53兴.
Therefore formation of clusters approaching the overlap volume fraction * could lead to dynamical arrest of the system at smaller values of the packing fractionthan pre-dicted by MCT 关6兴, where the cage effect suppresses the
dynamics when the particles already overlap significantly 共⬎*兲.
Moreover, clusters can induce in the samples an “effec-tive” polydispersity in the sample 关66兴 that suppresses the
underlying fcc phase. In addition, the absence of significant block copolymer exchange between micelles hampers the or-dering into the fcc phase. For f⬍70 on the contrary the glass transition is predicted for packing fractions well above the
crystallization boundary. Therefore this effect does not play an important role and we could observe crystalline phases.
We have presented a detailed investigation of single par-ticle properties and interactions of starlike PEP-PEO copoly-mer micelles. The micellar system was first characterized by SANS combined with contrast variation, in terms of single particle properties, determining the functionality and the core and shell radii as a function of DMF content of the solvent. It was shown that the shell contrast form factor of the micellar corona can be modeled assuming a starlike density profile. The starlike morphology of the micelles was also directly confirmed by comparison to form factor data of a corre-sponding 共same functionality兲 PB star polymer and evi-denced in a Kratky representation. On the basis of single particle properties we could therefore conclude that the mi-celles are an easily tunable system having a starlike architec-ture.
The interactions in the system were found to reproduce those observed for PB star polymers, as obtained by a direct comparison of the experimental structure factors of the two systems below, at and above the overlap concentration. Moreover, it was shown that the pair potential describing the interactions between star polymers correctly describes also the interactions between PEP-PEO micelles. Therefore we could conclude that PEP-PEO micelles are a model system for both single particle properties and interactions of real star polymers. Hence we used PEP-PEO micelles to investigate the phase diagram of real star polymers. The agreement be-tween experimental and theoretical phase diagram was found to be generally satisfactory, in particular the liquid-solid boundary is correctly reproduced in experiments for all func-tionalities. For f⬍70 the solid phase was identified as a bcc crystalline phase. The critical packing fraction for a liquid-to-bcc crystal transition for f⬍70 shows excellent agreement with theory. We suggest that the observed bcc phases are not homogeneous, rather coexisting with dynamically arrested regions which grow in size approaching the MCT glass tran-sition line. For f⬎70 the solid phase was identified as a dynamically arrested state. We suggest that the arrested state arises from dynamical frustration of the chain motions due to the confinement of the polymer chains of the corona when the particles start to overlap. This is in agreement with regu-lar star polymers with sufficiently dense corona. This effect was not taken into account in MCT calculations, but explains the early onset of gelation observed in experiments com-pared to theory. Moreover, we speculate that an effective polydispersity induced by cluster formation could prevent the occurrence of the equilibrium fcc crystalline phase.
We acknowledge the allocation of SANS beam time by Forschungszentrum Juelich 共FZJ兲, Institute Laue-Langevin共ILL兲, and Laboratoire Leon Brillouin 共LLB兲 and assistance during the SANS experiments by A. Radulescu
FIG. 10. 共Color online兲 Structure factors for samples in the glassy solid state for f = 82共䊊兲 and f =136 共䉱兲 at ⱖ*. Inset:
Dynamic frequency sweeps for a liquid共=0.03, 䊏兲 and a solid 共=0.035, 䉱兲 sample of hydrogenated PEP-PEO micelles in water.
共FZJ兲, P. Lindner 共ILL兲, and L. Noirez 共LLB兲. We acknowl-edge helpful discussions with C.N. Likos and F. Lo Verso. This work was supported by the Deutsche Forschungsge-meinschaft in the framework of the Transregio-SFB TR6. We
acknowledge also support from SOFT COMP: NoE Soft-Comp, Contract No. NMP3-CT- 2004-502235. E.Z. ac-knowledges support from MIUR-Prin and MCRTN-CT-2003-504712. MIUR
关1兴 C. N. Likos, H. Löwen, M. Watzlawek, B. Abbas, O. Jucknis-chke, J. Allgaier, and D. Richter, Phys. Rev. Lett. 80, 4450 共1998兲.
关2兴 G. S. Grest, L. Fetters, J. Huang, and D. Richter, Adv. Chem. Phys. 94, 67共1996兲.
关3兴 J. Stellbrink, J. Allgaier, M. Monkenbusch, D. Richter, A. Lang, C. N. Likos, M. Watzlawek, H. Löwen, G. Ehlers, and P. Schleger, Prog. Colloid Polym. Sci. 115, 88共2000兲.
关4兴 O. Juckniscke, Ph.D. thesis, Universität Münster, 1995 共unpub-lished兲.
关5兴 M. Watzlawek, C. N. Likos, and H. Löwen, Phys. Rev. Lett.
关6兴 G. Foffi, F. Sciortino, P. Tartaglia, E. Zaccarelli, F. Lo Verso, L. Reatto, K. A. Dawson, and C. N. Likos, Phys. Rev. Lett. 90, 238301共2003兲.
关7兴 E. Stiakakis, D. Vlassopoulos, C. N. Likos, J. Roovers, and G. Meier, Phys. Rev. Lett. 89, 208302共2002兲.
关8兴 K. Ishizu, T. Ono, and S. Uchida, J. Colloid Interface Sci. 192, 189共1997兲.
关9兴 D. Richter, O. Jucknischke, L. Willner, L. J. Fetters, M. Lin, J. S. Huang, C. Toporovski, and L. L. Zhou, J. Phys. IV 3, 3 共1993兲.
关10兴 J. Roovers, Macromolecules 27, 5359 共1994兲.
关11兴 I. W. Hamley, The Physics of Block Copolymers 共Oxford Uni-versity Press, New York, 1998兲.
关12兴 A. Halperin, Macromolecules 20, 2943 共1987兲.
关13兴 Y. Séréro, R. Aznar, G. Porte, J.-F. Berret, D. Calvet, A. Collet, and M. Viguier, Phys. Rev. Lett. 81, 5584共1998兲.
关14兴 E. Beaudoin, O. Borisov, A. Lapp, L. Billon, R. C. Hiorns, and J. Francois, Macromolecules 35, 7436共2002兲.
关15兴 F. Lafleche, D. Durand, and T. Nicolai, Macromolecules 36, 1331共2003兲.
关16兴 L. Willner, A. Poppe, J. Allgaier, J. Monkenbusch, P. Lindner, and D. Richter, Europhys. Lett. 51, 628共2000兲.
关17兴 R. Lund, L. Willner, J. Stellbrink, A. Radulescu, and D. Rich-ter, Macromolecules 37, 9984共2004兲.
关18兴 G. A. McConnell, A. P. Gast, J. S. Huang, and S. D. Smith, Phys. Rev. Lett. 71, 2102共1993兲.
关19兴 J. Bang, T. P. Lodge, X. Wang, K. L. Brinker, and W. R. Burghardt, Phys. Rev. Lett. 89, 215505共2002兲.
关20兴 T. P. Lodge, J. Bang, M. J. Park, and K. Char, Phys. Rev. Lett.
关21兴 I. W. Hamley, J. A. Pople, and O. Diat, Colloid Polym. Sci.
关22兴 M. Laurati, J. Stellbrink, R. Lund, L. Willner, D. Richter, and E. Zaccarelli, Phys. Rev. Lett. 94, 195504共2005兲.
关23兴 A. Poppe, L. Willner, J. Allgaier, J. Stellbrink, and D. Richter, Macromolecules 30, 7462共1997兲.
关24兴 R. Lund, Ph.D. thesis, Universität Münster, 2004 共unpub-lished兲.
关25兴 R. Lund, L. Willner, J. Stellbrink, P. Lindner, and D. Richter,
Phys. Rev. Lett. 96, 068302共2006兲.
关26兴 R. Lund, L. Willner, D. Richter, and E. Dormidontova, Mac-romolecules 39, 4566共2006兲.
关27兴 G. D. Smith, D. Y. Yoon, R. L. Jaffa, R. H. Colby, R. Krish-namoorti, and L. J. Fetters, Macromolecules 29, 7602共1996兲. 关28兴 M. Laurati, Ph.D. thesis, Universität Münster, 2005
关29兴 P. Lindner and Th. Zemb, Neutrons, X-Rays and Light: Scat-tering Methods Applied to Soft Condensed Matter 共North-Holland, Amsterdam, 2002兲.
关30兴 M. Kotlarchyk and S. H. Chen, J. Chem. Phys. 79, 2461 共1983兲.
关31兴 J. S. Pedersen, J. Chem. Phys. 114, 2839 共2001兲.
关32兴 J. S. Pedersen and C. Svaneborg, Curr. Opin. Colloid Interface Sci. 7, 158共2002兲.
关33兴 V. Castelletto and I. W. Hamley, Curr. Opin. Colloid Interface Sci. 7, 167共2002兲.
关34兴 C. Svaneborg and J. S. Pedersen, Macromolecules 35, 1028 共2002兲.
关35兴 S. Förster and C. Burger, Macromolecules 31, 879 共1998兲. 关36兴 G. Beaucage, J. Appl. Crystallogr. 28, 717 共1995兲.
关37兴 F. J. Rogers and D. A. Young, Phys. Rev. A 30, 999 共1984兲. 关38兴 M. Watzlawek, H. Löwen, and C. N. Likos, J. Phys.: Condens.
Matter 10, 8189共1998兲.
关39兴 F. Lo Verso, M. Tau, and L. Reatto, J. Phys.: Condens. Matter
关40兴 E. Zaccarelli et al., Phys. Rev. Lett. 95, 268301 共2005兲. 关41兴 C. Mayer, E. Stiakakis, E. Zaccarelli, C. N. Likos, F. Sciortino,
H. Löwen, P. Tartaglia, and D. Vlassopoulos, Rheol. Acta 46, 611共2007兲.
关42兴 A. Lang, G. Kahl, C. N. Likos, H. Löwen, and M. Watzlawek, J. Phys.: Condens. Matter 11, 10143共1999兲.
关43兴 P. Kumar, S. V. Buldyrev, F. Sciortino, E. Zaccarelli, and H. E. Stanley, Phys. Rev. E 72, 021501共2005兲.
关44兴 C. Sommer, J. S. Pedersen, and P. C. Stein, J. Phys. Chem. B
关45兴 B. Hammouda, D. Ho, and S. Kline, Macromolecules 35, 8578 共2002兲.
关46兴 J. S. Pedersen, D. Posselt, and K. Mortensen, J. Appl. Crystal-logr. 23, 321共1990兲.
关47兴 J. S. Higgins and H. C. Benoit, Polymers and Neutron Scatter-ing共Oxford University Press, New York, 1994兲.
关48兴 L. Willner, O. Jucknischke, D. Richter, J. Roovers, L. L. Zhou, P. Toporowski, L. Fetters, J. Huang, M. Lin, and N. Hadjichris-tidis, Macromolecules 27, 3821共1994兲.
关49兴 D. Richter, B. Farago, J. S. Huang, L. J. Fetters, and B. Ewen, Macromolecules 22, 468共1989兲.
关50兴 D. Richter, B. Farago, L. J. Fetters, J. S. Huang, and B. Ewen, Macromolecules 23, 1845共1990兲.
关51兴 H. Benoit, J. Polym. Sci. 11, 507 共1953兲.